Electrochemical characterisation of the porosity and corrosion 2019-08-28¢ ...
Embed Size (px)
Transcript of Electrochemical characterisation of the porosity and corrosion 2019-08-28¢ ...
Surface & Coatings Technology 202 (2008) 5092–5102
Contents lists available at ScienceDirect
Surface & Coatings Technology
j ourna l homepage: www.e lsev ie r.com/ locate /sur fcoat
Electrochemical characterisation of the porosity and corrosion resistance of electrochemically deposited metal coatings
F.C. Walsh a,⁎, C. Ponce de León a, C. Kerr b, S. Court c, B.D. Barker c
a Electrochemical Engineering Laboratory, Energy Technology Research Group, School of Engineering Sciences, University of Southampton, Highfield, Southampton SO17 1BJ, United Kingdom b Tin Technology Ltd., Unit 3, Curo Park, Frogmore, St. Albans, Herts. AL2 2DD, United Kingdom c Applied Electrochemistry Group, University of Portsmouth, St. Michael’s Building, White Swan Road, Portsmouth PO1 2DT, United Kingdom
0257-8972/$ – see front matter © 2008 Elsevier B.V. Al doi:10.1016/j.surfcoat.2008.05.008
⁎ Corresponding author. E-mail address: F.C.Walsh@soton.ac.uk (F.C. Walsh).
A B S T R A C TA R T I C L E I N F O
Electrochemical techniques f
Received 30 November 2007 Accepted in revised form 8 May 2008 Available online 17 May 2008
Keywords: Corrosion resistance Corrosion testing Current vs. time Linear polarisation resistance Electroless nickel coatings Polarisation curves Porosity Tafel extrapolation
or the assessment of porosity in electrodeposited metal coatings are reviewed. The determination of porosity and corrosion, resistance is illustrated by electrochemical data from three coating/ substrate systems namely: electroless nickel on aluminium and steel and immersed gold coatings on an electroless copper-plated ABS polymer. Nickel coatingswere up to 24 μm thick while gold deposits had thickness between 75 and 190 nm. Tafel extrapolation and linear polarisation resistance methods were used to determine the corrosion rate of the coated substrates. The aluminium samples were tested in 5%w/v (0.85mol dm−3) NaCl, while coated steel and ABS samples were immersed in 0.125 mol dm−3 H2SO4 and 0.1 mol dm
−3 NaBH4, respectively, at 295 K. Current vs. time curves and anodic polarisation behaviour have also been considered.
© 2008 Elsevier B.V. All rights reserved.
Through-porosity is an important parameter that should be assessed to estimate the life expectancy of coated components and their quality. Porosity in the coating is strongly related to the corrosion resistance of the substrate . For example, a galvanic cell can be formed in an electroless nickel (EN) coating on aluminium or steel immersed in an acid. This galvanic cell promotes substrate dissolution and hydrogen evolution (or oxygen reduction) on the nickel coating. The noble nickel coating can also be dissolved in the acidic environment increasing the pore size and number, accelerating localised corrosion of the (base) substrate.
In the case of electroless coatings, the corrosion resistance depends on the phosphorus content ; for example, high corrosion resistance in acidic environments have been achieved at N10% phosphorus content while low (b4%) phosphorus content coatings tend to perform well in alkaline electrolytes  and at elevated temperatures .
For comparable pre-treatment schedules, the porosity of EN coatings has been shown to be much lower than that in nickel electrodeposits from a Watts bath . The porosity of EN coatings is linked to a number of factors that decrease the corrosion resistance of the coated substrate, such as: aged baths , inadequate substrate pre- treatment [7,8], surface roughness [9–11] and coating microstructure
l rights reserved.
. Porosity can be affected by heat treatment due to the shrinking of the coating when its structure changes from amorphous to crystalline during the curing process, exposing part of the substrate .
1.1. Porosity tests
There are numerous chemical and electrochemical porosity tests in the literature. Chemical porosity tests include neutral and acetic acid salt spray, sulfur dioxide exposure, the use of a ferroxyl indicator and corrodkote corrosion tests [10,14]. Such tests are designed to attack the substrate revealing the corrosion occurring through the pores. However, corrosion products could block the pores and give false readings while very fine pores are hard to penetrate by the electrolyte and may be missed. These tests often take a long time and visual results can be difficult to quantify and reproduce . In contrast, electrochemical technologies can be rapid and more reliable. A classical example is the electrographic test where a current is passed between the test specimen (anode) and an inert cathode. An absorbent paper soaked in an electrolyte containing a colorimetric indicator is sandwiched between the two electrodes. The current reveals coloured areas on the paper due to the reaction between the indicator in the electrolyte and the dissolved metal ions from the test specimen showing the location of the pores. A disadvantage is that very small pores can be missed with this technique; it is also important to chose appropriate electrolyte (and indicator) composi- tion and the duration of the test. Other electrochemical tests, such as Tafel extrapolation, cyclic voltammetry, linear polarization resistance
http://dx.doi.org/10.1016/j.surfcoat.2008.05.008 http://www.sciencedirect.com/science/journal/02578972 mailto:F.C.Walsh@soton.ac.uk
Fig. 1. Log–log plot of percentage porosity vs. coating thickness for electroless nickel deposits onsteel in0.125moldm−3H2SO4at295K.Dataobtainedbycyclicvoltammetry.●)Nahléet al. ; and○) recent data obtained by Walsh et al. [unpublished work].
5093F.C. Walsh et al. / Surface & Coatings Technology 202 (2008) 5092–5102
and corrosion potential monitoring, are more quantitative and can be performed rapidly with standard electrochemical instrumentation [16–18]. Such techniques have been used to determine the percentage through-porosity in electroless nickel coatings on steel and alumi- nium substrates [19–22].
Electrochemical methods can be used to expose the underlying substrate in a carefully chosen electrolyte. An appropriate electrolyte will allowcontactwith the substrate throughpores in thedeposit andwith the coating material. The two metals form a bimetallic corrosion cell. If the coating is noble respect to the substrate, thedeposit shouldbepore-free to avoid a high cathode to anode area ratio, which can lead to intense, localised corrosion of the substrate. This is especially true for thin immersion deposits. Continuous electroless deposition of metal may slowly fill any pores left in previous coating layers .
In many cases, the general relationship between the porosity (P) and a uniformly deposited coating of thickness (x) takes the form :
P ¼ Axn ð1Þ where A and n are empirical constants that depend on pre-treatment, plating time and process conditions . Fig. 1 shows an example of the
Table 1 Direct current (d.c.) electrochemical techniques considered in this paper and their features
Technique Principle Example Advantages
Current density vs. time, j vs. t at E
Measure the dissolution j of coated samples at a fixed potential, E
Immersion deposits of Ni on steel
The curve yields the metal reflecting the r integrity of the coatin
Anodic polarisation, E vs. log j
Potential sweep to a value≈2 V anodic to the Ecor value
Ni on mild steel
Porous and non-porou behaviour. Time to per
Tafel behaviour, E vs. log j
Potential sweep to a value ≈0.15 V either side of Erest or Ecor. Corrosion data can be deduced
Electroless Ni on mild steel
Corrosion measurem Typically 30 min to c
Potential vs. time, Ecor vs. t
Potential within a given environment over time
Electroless Ni on pyrene steel
Non-porous coatings compared to porous.
LPR, E vs. I Potential sweep to a value of ≈0.05 V either side of Erest or Ecor
Electroless Ni on Al or Ni on Fe
Rapid (10 min) repro rates
Cyclic voltammetry E vs. J
Potential sweep from −0.5 to +0.5 back to −0.5 V vs. SCE
Electroless Ni coating on Al
Rapid (10 min) simpl instrumentation
relationship between percentage porosity and deposit thickness. The porosity was determined by cyclic voltammetry carried out on nickel- coated steel samples. The charge under the anodic peaks when the potential was swept towards negative values was measured for different thickness of nickel coated samples. The potential range and the electrolyte selected are such that anodic dissolution of the substrate occurs but nickel dissolution is negligible or occurs outside the potential range, at more positive potentials. The charge under the anodic peak without nickel coating was considered to represent 100% porosity while the charge exhibited by the samples with nickel coating was linearly correlated to the percentage of porosity . The log–log plot of percentage porosity vs. nickel deposit thickness corresponds to the logarithmic form of Eq. (1):
log P ¼ log Aþ n log x: ð2Þ
Such a plot shows reasonable linearity over a thickness range between 0.2 and 6 μmwith a correlation coefficient, r2 of 0.997. If x has units of μm, the values of the constants A and n are 12 and −1.35, respectively. The size, geometry and chemical homogeneity of the pores are not taken into account in this equation but it provides a reasonable approximationof the porosity over awide range of coating thickness, for a uniform thickness specific coating substrate-test protocol.
2. Electrochemical techni